Guideline for Welding P(T) 91
William F. Newell, Jr., PE*
Factors affecting use, development, and procurement of Modified Grade 91 welding
consumables for heavy wall applications are the focus of this report. Differences in technical approach between domestic and European producers and users are provided, particularly in composition variances. Prior and current activities are highlighted as well as progress to date in obtaining suitable fabricated wires with acceptable mechanical and operational properties.
The effects of composition, post weld heat treatment times and temperatures plus practical implementation factors as they relate to creep and toughness are examined. Availability and procurement considerations are also discussed. As we learn more about this alloy, it is becoming clear that P(T)91 should not be treated as just another CrMo steel. The alloy requires considerable care during joining to assure acceptable long term properties. (1)
2.0 INTRODUCTION (2-11)
Development of the Grade 91 or 9 chromium - 1 molybdenum steels microalloyed with vanadium, niobium(columbium) and controlled nitrogen is the result of research conducted at the Oak Ridge National Laboratory (ORNL) for the Clinch River Breeder Reactor and later carried out by Combustion Engineering and others during the late 1970’s. However, the
“super 9 chrome” alloys were initially evaluated for power boiler use between 1955 and 1960 at the Center for Metallurgical Research of Liege in Belgium. This early work resulted in a 9Cr-2Mo alloy with additions of niobium and vanadium. A parallel effort, but for different reasons, was conducted by the Timken Corporation (USA) concerning use of the alloy family for bearing applications.
The high temperature creep resistance of the generic 9Cr 2Mo alloy appeared ideal for increasing operating temperatures and efficiency plus reduction of wall thickness for many fossil fueled power applications. IlectricitJ de France approved a product produced by Vallourec (France) named EM12 in 1964 for use in superheater and reheat superheater applications up to temperatures of 620o C (1148oF). Approval was based on creep rupture tests of 760,000 hours on nine commercial heats. As of 1978, test data up to 200,000 hours was available. EM12 was also a candidate in 1978 for steam generator components in the European Fast Breeder Program. Even though EM12 provides satisfactory service in superheater tubing, the duplex structure results in low impact strength thus limiting the
material to use in thin sections. Over 9,000 tons of EM12 tubes have been installed, with many still in use on a world wide basis.
In the late 1960’s, German steel makers developed a 12 Chrome steel grade for high temperature applications to compete with EM12. This material, X20CrMoV12 1, was commonly referred to as “X20”. The primary advantage of the X20 material was its
martensitic structure which permitted use in heavy sections or thick walled piping systems.
*W. F. Newell, Jr. is a Co-Founder of Euroweld, Ltd. and President of W. F. Newell & Associates, Inc.
important, X20 exhibited poor weldability due to of its elevated carbon content. Other
competitive alloys such as the Swedish HT9 and Japanese HCM 9M were produced, but were not as widely used as EM12 or X20.
In 1974, a task force was initiated by the US Department of Energy (DOE) to select materials for the LMFBR (Liquid Metal Fast Breeder Reactor) Program. The Oak Ridge National Laboratory (ORNL), assisted by Combustion Engineering, initiated a program to develop a 9Cr-1Mo steel that included all of the advantages of the EM12 and X 20 alloys plus eliminated the disadvantages. The orginal service temperature called for this material to provide strength at 5120C (9700F) and toughness of 54J (40 ft-lbs) at room temperatue for selected liquid sodium coolant components.
Creep resistance, weldability and the ability to commercially produce the alloy were
considerations. Toughness was the primary consideration. By 1980, over 100 base metal test heats had been formulated and tested. The resulting composition of the Modified 9Cr-1Mo (later T/P91) is shown in Table 2. Multiple refining operations in the steel making practice were found to be required to achieve the controlled composition.
Table 2. Summary of Heat Treatment and Mechanical Property Requirements for Modified 9Cr-1Mo Steels (13)
The first set of Modified 9Cr-1Mo test tubes were installed in May 1980 in superheater sections of the TVA Kingston Unit 5 station, replacing TP321 stainless steel tubing.
Modified 9Cr-1Mo was recognized for tubing by ASTM as A213, Grade T91, in 1983. Use of the material for piping and headers was approved by ASTM (and ASME) as A/SA-335, Grade P91 in 1984. A European (German) equivalent is DIN 1.4903, Grade or Type X10
Figure 1. illustrates a comparison of wall thickness for various alloys for a given elevated temperature, pressure and European allowable strengths. Note that nearly a 2:1 reduction in wall thickness (61mm versus 132mm) is possible where Modified Grade 91 or P(T)91 (herein referred to as P91) is used in place of P22 material. The material provides an increase of 44 to 170% in allowable strength in the 5100C (9500F) to 5930C (11000F) temperature range. The oxidation limit is also 380C (1000F) above typical Grade 22 materials. Grade 91 also offers higher allowable strengths over type 304H up to 6100c (11300F).
Figure 1. Comparison of Thickness and Weight using P(T)91 versus P(T)22.(38) Thousands of tons of P91 materials are in use worldwide. Until about 1998, most installations or retrofits, however, have not been in the United States. Three major reasons were initially cited by domestic fabricators and end users for not using the P91 material:
1. The material is not readily available or is a special order (when the “ORNL Composition” is specified)
2. All welds require post weld heat treat, regardless of thickness or diameter
3. Installation and heat treatment of dissimilar weldments (e.g., P22 to P(T)91) can be complex in either shop or field applications.
Except for some selected Japanese variations, a consensus was observed concerning the base material, regardless of product form. The ORNL base metal composition was and is being produced and used in accordance with nationally recognized material specifications. Weld metal composition usage and specification, on the other hand, exhibit two distinctly different schools of thought: low nickel (0.4 max. per ORNL/CE) versus high nickel (~ 0.6 to 0.8 in Europe, plus tolerance for up to 0.5 silicon).
Currently, most of the consumables for welding P(T)91 components (hereafter referred to as P91) are produced overseas, due to greater use, and vary from the original ORNL
recommendations. Increased levels of nickel and silicon or nickel + manganese limitations are observed over those in the ORNL specifications. Nickel is elevated to enhance toughness, but Ni+Mn limitations are utilized to ensure that the AC1 transformation temperature is maintained at a level sufficient to permit proper tempering. Minor increases in the silicon level are desired
European produced material occasionally fell within the AWS/ASME filler metal specifications for “B9” (Modified 9Cr-1Mo) classifications. Material required to meet the “ORNL”
specification was usually a special order.
Today consumables meeting “B9” specifications (“ORNL”) are available from a variety of sources. Procurement of standard, commodity type consumables such as E7018, E308L-15 or ER316 is rather straightforward. However, when weld metal toughness, properties after post weld heat treatment, specified ferrite criteria, hardness, or other out-of-the-ordinary
requirements are needed, communication between the purchaser and supplier becomes critical.
This is especially the case with consumables for welding the 9CrMoV or P(T)91 materials.
P(T)91 should not be treated as just another CrMo steel. The alloy requires considerable care during joining to assure acceptable long term properties. (1) Table 1. illustrates some of the major differences when compared with a traditional CrMo material.
Table 1. Comparison of Important Variables when Welding P(T) 22 versus P(T) 91.
Base Metal Variable
P(T) 22 P(T) 91
Preheat Always Always !
PWHT Sometimes (some code exemptions) Always ! Normalize & Temper
(after bending or cold working)
Sometimes Always ! (> 18% strain)
Certified Material Test Report Rarely (not normally required) Always ! (PWHT < AC1)
Toughness Requirements Rarely (not normally required) Always !
Post Bake Rarely (not normally required) Always ! (except GTAW)
Cool < 1000C before PWHT No (not required) Yes (pending further study)
Bead Sequence Rarely (not normally required) Always ! (interbead tempering needed)
Purge No (not normally required) Always ! (material will sugar)
3.0 BASE MATERIAL PROPERTIES
3.1 Base Metal Mechanical Properties (1,6,9,35,36)
Base metal material properties are directly influenced by the composition and subsequent heat treatment operations. Typical properties for selected P(T) 91 product forms are shown in Table 2. Comparison of P(T) 91 with P(T)22 and Type 304H austenitic stainless steel are provided for themal conductivity in Figure 2 and coefficient of linear expansion in Figure 3.
Data on modulus of elasticity is shown in Figure 4. P(T)91 is becoming a material of choice because of its better thermal conductivity and lower coefficient of linear expansion.
Figure 2. Thermal Conductivity among various alloys. (9)
Figure 3. Mean coefficient of linear expansion comparison. (9)
Because chemical composition may vary among heats of material, transformation temperatures will also vary. The AC1 (lower critical) typically ranges between 8000C (14720F) and 8300C (15260F), but values as low as 7850C (14450F) have been observed. The AC3 (upper critical) has been found to range from 8900C (16350F) to 9400C (17250F). A continuous cooling temperature diagram for a selected P(T) 91 material is shown in Figure 5. Note that these values do NOT apply to weld metal.
This material is generally used in a normalized and tempered condition. Upon cooling from the austenitizing temperature to room temperature, the P(T) 91 structure transforms totally into martensite even with varying cooling rates. The maximum hardness of the martensite is characteristically less than 450 HV. The Ms (martensite start) temperature is normally around 4000C (7500F). The end of the martensite transformation, Mf, usually lies above 1000C (2100F) and will vary depending upon prior austenite grain size.
Figure 4. Modulus of elasticity versus temperature. (9)
Figure 5. Continuous cooling transformation diagram for P(T) 91.
Heat treatment(s) of base material is selected to provide the best compromise between creep rupture strength, hardness and toughness. To achieve this compromize, material undergoes a quench and temper sequence. The material is typically normalized between 10400C (19000F) and 10800C (19800F) to dissolve most carbides without creating objectionable grain growth.
The product form is then tempered between 7500C (13800F) and 7800C (14350F) to allow carbides to precipitate within the martensitic structure and soften the material. Yield strength, tensile strength and hardness will usually decrease while toughness increases as tempering temperatures approach the AC1. Tempering above the AC1 results in increased strength and
decreased toughness due to the formation of fresh martensite, but also significantly reduces creep rupture properties.
Heat treatments outlined herein will produce a structure of tempered martensite with
preciptiation of M23C6 carbides and vanadium/niobium rich carbo-nitrides. These precipitates tend to improve creep rupture strength via precipitation hardening. The M23C6 carbides predominately stabilize the martensitic structure.
Welding & Forming
Welding of this material must be conducted with preheat and followed by post weld heat treatment (PWHT) to ensure that ductility has been restored in the weld metal and weld heat- affected zone. Adequate toughness must be present, even after PWHT, to ensure that the material will not be damaged in transit, during installation or shut down conditions. Experience over the last decade has shown that where the base metal is subjected to cold bending strains over 18%, the material must be normalized and tempered. One original equipment
manufacturer performs a normalize and temper on all items that have seen cold bending and do so on the entire component. Localized normalizing and tempering has been found to be
unacceptable. Normalizing and tempering may be the only way to completely eliminate the effects of a weld heat-affected zone.
Further, where thermal straitening is implemented, caution must be observed to not encroach on the lower critial (AC1) temperature of the materal. If this is exceeded, the component must again be normalized and tempered. Some authorities make these additional heat treatments mandatory. (1)
3.2 Base Metal Composition
The composition of Modified 9Cr-1Mo base material in accordance with ASME/ASTM SA/A213, Grade T91, SA/A-335, Grade P91 or DIN 1.4903 Grade X10 CrMo.V.Nb 91 is provided in Table 3. The composition now used was derived from the ORNL program.
4.0 WELDMENT PROPERTIES
The weld deposit composition is designed to be as close as possible to the parent steel while maintaining mechanical properties and weldability. Early attempts to match base metal composition resulted in lower toughness when tempered within reasonable time and temperature cycles - typically 2 to 3 hours at 750 to 7600C (1382-1400 0F).
Examples of typical properties at room temperature (RT) for P91 all weld metal versus weldments are provided in Table 4. In addition to tensile, yield strength and hardness, this material must provide creep resistance at elevated temperatures as well as exhibit reasonable
challenge because measures for enhancing one property normally adversely affects the other.
Table 3. Comparison of “Grade 91 Modified” Weld Metal Compositions (13-17)
Element P/T91 Steel
Gr. 91 AWS A5.28-96
Gr. 91 AWS A5.23-97
Gr. 91 AWS A5.5-96
Gr. 91 BS EN 1599:1997
Gr. 91 EN 12070:1996
Process N/A GTAW SAW SMAW SMAW GTAW
C 0.08/0.12 0.07/0.13 0.07/0.13 0.08/0.13 0.06/0.12 0.07/0.15
Mn 0.30/0.60 1.25 1.25 1.25 0.40/1.50* 0.4/1.5*
P 0.020 0.010 0.010 0.01 0.025 0.020
S 0.010 0.010 0.010 0.01 0.025 0.020
Si 0.20/0.50 0.15/0.30 0.30 0.30 0.60 0.6
Cr 8.00/9.50 8.00/9.50 8.00/10.00 8.00/10.50 8.0/10.5 8.0/10.5
Mo 0.85/1.05 0.80/1.10 0.80/1.10 0.85/1.20 0.80/1.20 0.80/1.20
Ni 0.40 1.00 1.00 1.00 0.40/1.00* 0.4/1.0*
V 0.18/0.25 0.15/0.25 0.15/0.25 0.15/0.30 0.15/0.30 0.15/0.30
N2 0.03/0.07 0.03/0.07 0.03/0.07 0.02/0.07 0.02/0.07 0.02/0.07
Nb 0.06/0.10 0.02/0.10 0.02/0.10 0.02/0.10 0.03/0.10 0.03/0.10
Single values are maximums. * Ni + Mn < 1.5 ** Draft in Review.
Major differences between base metal and weld metal are highlighted in bold type.
Table 4. Typical Grade 91 All Weld Metal Mechanical Properties at Room Temperature.(2, 17-19)
Process Deposit Ultimate, MPa (Ksi)
SMAW1 All Weld Metal
820 (120) 700 (102) 65 (47) 2403
Weldment 6985 (102) N/A 54 (39) N/A
GTAW1 All Weld Metal
750 (109) 660 (87) 147(109) 2403
Weldment 7035 (103) N/A 199 (144) N/A
FCAW Metal Core3 75Ar-25CO2
Metal 8506 (124) (116) (111)
7206 (105) (97) (92)
32 (23) (23) (23)
2603 246 246
Weldment N/A N/A N/A N/A
SAW3 All Weld Metal
7201 (105) 6101 (89) 60 (44) 2401
Weldment 6574 (96) N/A 54 (39) N/A
Notes: 1. PWHT: 760oC/2hr 2. PWHT: 765oC/2hr 3. PWHT: 760oC/4hr 4. PWHT 7600C/2hr 5. Fracture in base metal. 6. PWHT: 7550C/3hr
4.1 Tensile Properties
Typical ultimate and yield strength, elongation, and hardness values for all weld metal and weldments with various welding processes used to join Grade 91 are illustrated in Table 4.
4.2 Creep Considerations (2-18)
Test results have shown that creep failure of welded joints in P91 steel welded with matching or near-matching weld metals occurs in the parent material. (9-12, 15-19) The
reduction in transverse creep strength of P91 weldments is typically about 20%. However, creep considerations do not characteristically become relavent until the operating
temperature is greater than 1,0500F (5660C).
Figure 6. illustrates stress-rupture properties for P91 base metal and representative weldments. A number of observations can be made:
• with the possible exception of very short duration tests, all the weldments lie below the average claimed by ORNL for P91 steel base metal
• in longer duration tests, weldment properties show increasing divergence from the P91 base metal
• all the weldments indicate similar behavior. It should be noted that failure location in cross-weld tests is normally at the outer boundary of the visible HAZ. This region is partially re-austenitized by re-heating within the intercritical temperature range during the welding thermal cycle where most of the carbon and nitrogen is precipitated from solution. Further recrystallization of the transformed microstructure during PWHT then produces a relatively soft martensite which lacks the carbo-nitride grain strengthening essential for creep resistance. This weakened zone where “Type IV”
creep failure occurs is characteristic of all creep resisting CrMo steels. Figure 7. shows a typical hardness survey with a hardness almost 40HV below the base material
Figure 6. Creep Properties of Typical P91 Weldments. (16)
Figure 7. Representative Microhardness Across a P91 Weldment. (18)
Since Type IV failure is typical for cross-weld creep tests (except possibly for very high stress/short duration tests), the actual role of the weld metal creep performance could be
considered as having little practical significance, except that it should perform at least as well as the HAZ region. Some authorities accept this observation. (11,16)
However, there are two other contrasting opinions concerning the influence of weld metal creep properties on the overall behavior of weldments or the possibility that weld metal behavior might be optimized in an attempt to delay the onset of Type IV failure:
• One proposal is that the weld metal should actually be weaker than the parent material and comparable with the type IV zone creep strength. (16)
• The alternative proposition is that the relatively wide weld zone should have a strength comparable to the base material so that less strain will be transferred to the narrow type IV zone and failure will therefore be delayed. (16)
Early work in the USA and recently discussed by Zhang, et al, (18) indicated that reducing niobium content to levels as low as 0.02 wt. % resulted in significantly tougher weld metal than the parent base metal (0.06 to 0.10 wt. %). Testing has also shown that a lower limit of 0.04 wt. % niobium is necessary to maintain satisfactory creep resistance. The accepted range is controlled to within 0.04 to 0.07 wt. %. (7,10,16)
Encouraging creep rupture results have been observed with reduced niobium levels, down to 0.025 to 0.03, from selected FCAW wires. The higher rupture stress of the FCAW weld metal is believed to be caused by the presence of residual titanium. Titanium forms stable
carbonitrides like niobium, a positive influence was anticipated, and the intentional reduction of Nb was justified.
No previous reports highlighting the effects of Ti in P91 weld metal are available, but a similar level (200ppm Ti) was found to have no effect on 650°C rupture life in a low nitrogen 11%Cr rotor steel, and contrary to the weld metal here, fracture appearance transition temperature (FATT) was noticeably reduced. Early results suggest that this approach may even provide enhanced performance as shown in Figure 8.
Greater possible importance is the pick up of titanium into the weld metal which provides a further strong carbide former and provide more matrix strengthening. FCAW weld metals are generally about 5-10% stronger at ambient temperature than weld metals from SMAW and SAW processes and are similar to those of GTAW deposit after similar PWHT. The corresponding toughness is generally lower. To mitigate the effects of Ti pick-up (typically 0.02-0.04%Ti), the level of Nb is deliberately controlled to the minimum consistent with meeting weld metal specifications. A small proportion of this Nb is also derived from the rutile flux system.
It must also be cautioned that Grade 91 material is still susceptable to Type IV cracking, thus, it must be sized to properly accommodate performance in service. Both stress and operating temperature must be considered. There is general agreement that the failure mode of
weldments is ultimately controlled by HAZ behavior, but currently there is no consensus as to the optimum choice of weld material properties to delay such failure and ultimately extend component life. This is particularly important where the design may consider longitudinal welds. In this case, some codes require derating the material an additional 20 to 40 percent to accommodate the elevated stresses associated with a longitudinal weld. Creep resistance behavior was generically categorized by EPRI (13-15), ORNL (20), Thyssen (2), and corroborated by others (16,25, 36, 38) as shown in Table 5.
Table 5. Grade 91 Weldment Performance Test Behavior. (2,3,10,11,13-16, 20, 25, 36, 38) Temperature, oC (oF) Performance – Creep Results
550 (~960) Base Metal, Weld and HAZ Have Comparable Properties
600 (~1050) Base Metal and Weld Have Similar Properties; HAZ ~ 20% Less 650 (~1200) Weld and HAZ Have Slightly Inferior Properties
Figure 8. Larson-Miller plot of all-weld metal stress-rupture test results at 550-660°C for FCAW and SMAW (19)
4.3 Toughness Considerations
Four factors have a significant influence on weld metal toughness:
• Post weld heat treatment time and temperature
• Welding process
• Microstructural effects (heat input, bead size, sequence and welding position)
• Toughness Testing Temperature
It has been argued that weld metal toughness is an irrelevant consideration for components which are designed to operate at temperatures in the range 500-6000C (932-11120F) - far above the range at which any possible risk of fast brittle fracture could occur. However, there are situations where components might be pressurized or loaded at ambient temperatures
during hydrostatic testing, construction, or start-up. To handle such conditions, most OEM’s and fabricators consider that the weld metal should have a minimum toughness at + 200C (680F). The American Welding Society (AWS) filler metal specifications do not specify impact requirements for "-B9" filler metals, but the non-mandatory appendix to AWS A5.5-96
(covered electrodes) proposes that a suitable test criterion should be agreed upon between the purchaser and supplier. Conversely, the recently introduced European specification EN 1599:
1997 requires a minimum average of 47J (34.7 ft-lbs.) with a minimum single value of 38J at + 200C (28 ft-lbs @ 680F). These values coincide with some internal corporate specifications from those whom have imposed toughness criteria and required values in the range 20-50J at 200C (14.8-36.9 ft-lbs @ 680F) after PWHT. Determination of adequate toughness became an issue, particularly because of early work with the FCAW process.
Table 6. CTOD and KQ values of Supercore F91 weld metal. (19) PWHT procedure Test temperature, °C CTOD, mm KQ, MPa
m 0.021 75.10 0.018 61.80 20
0.030 76.79 0.029 69.26 0.021 55.75 760°C×2h+FC
To answer the above question about the toughness of FCAW, a study was commissioned to calculate the maximum tolerable flaw sizes using critical assessment procedures set out in BS7910 (33,34). The model chosen was that of a fabricated header of 450mm (~18 in.) outside diameter and 50mm (~ 2 in.)wall thickness. The design conditions were 176 bar (2552 psi) at 580°C (10760F) with hydrotest conditions of 1.25 times design pressure at ambient temperature. This ensured that a comparison could be made between the FCAW and SMAW weld metals under similar conditions. (18,19)
To assess the worst toughness situation, the lowest measured CTOD value, namely δC = 0.018mm at 20°C, was used in the BS 7910 (33,34) calculations. The results indicate a maximum tolerable surface flaw size of 125mm in length and 12.5mm in depth for a
longitudinal seam weld, i.e. equal to ¼ of the wall thickness. The results are shown in Table 6.
Comparing the above data with those achieved by other flux shielded processes, namely SMAW and SAW (2), the FCAW deposit, as expected, produced somewhat lower impact energy values. However, as illustrated by Figure 9, slightly higher PWHT temperature or longer soaking times are normally beneficial for improving impact toughness.
Figure 9. The effect of PWHT on FCAW weld metal toughness. (19)
4.3.1 Weld Metal Composition & Delta Ferrite
Various approaches to the weld metal composition have evolved since the original ORNL/CE project funding efforts from EPRI and others. Table 3 illustrates variations as they exist today between the USA and Europe. Although the Japanese will supply products that meet many of these compositions, they have modifications with increased tungsten additions, for example.
In general terms, those elements which are beneficial for improving creep performance are detrimental in terms of toughness, for example: Nb/Cb, V and to a lesser extent N and Si. A balanced composition or alloy that restricts delta ferrite formation but results in a fully martensitic microstructure helps to contribute both-optimum toughness and creep performance.
In the design of the flux cored wire, the deposit composition was aimed to be as close as possible to the requirements of the corresponding SMAW weld metal (e.g. AWS E9015-B9).
The next revision of AWS A5.29 specification for low alloy flux cored wires will include this grade, and the expected classification for an all-positional wire will be E10XT1-B9. AWS specifications are ultimately included in Section II Part C of the ASME Boiler and Pressure Vessel Code. (32)
Table 7. presents the typical all-weld metal composition of a selected FCAW deposit. This composition is typical of a deposit made using welding grade Ar-20%CO2 shielding gas.
However, selected FCAW wires are formulated to work with either Ar plus15-25%CO2 or 100%CO2 shielding gases. Only minor changes in composition are typically observed.
Table 7 . Chemical composition of a typical FCAW weld metal.
Elements C Mn Si S P Cr Ni Mo Nb V N
wt% 0.10 0.8 0.3 0.010 0.015 9.5 0.6 1.0 0.03 0.20 0.05
To obtain a proper balance between fracture toughness, creep-rupture strength and resistance to long term embrittlement, the alloy composition and residual elements must be controlled to provide a single phase microstructure and avoid delta ferrite. The ORNL/CE programs found that by keeping the Chrome Equivalent (CE = Cr + 6Si + 4Mo + 1.5W + 11V + 5Cb + 9Ti + 12Al – 40C – 30N – 4Ni – 2Mn – 1Cu), as adjusted per their work, below 10, the tendency to form delta ferrite is reduced. This number is not absolute, but provides a good guideline since elevated delta ferrite in this material reduces its toughness. Even materials with a CE between 10 to 12 exhibited adequate toughness provided that the delta ferrite does not exceed five (5) percent.
It is widely recognized that nickel can be useful for improving weld metal toughness. The addition of a controlled level of nickel is beneficial for two reasons. Nickel lowers the AC1 transformation temperature bringing this closer to the post weld heat treatment (PWHT) temperature and this improves the response to tempering. It also eliminates the possibility of residual delta ferrite being present which is undesirable because of its poor creep resistance and potentially adverse effect on toughness. However, excessive levels of nickel, exceeding 1% are also detrimental. The AC1 may be so low that PWHT at the top end of the
temperature range could cause some austenite to form which in turn transforms to fresh untempered martensite on cooling. Most fabricators prefer to perform PWHT at least 50oF (320C) below the transition temperature to allow room for minor temperature excursions.
Excessive nickel also contributes to degradation of creep properties by changing the optimum long-term evolution of carbide precipitation during service. Nickel is therefore usually
controlled in the range 0.4 - 1.0 wt.% in Europe.
The original ORNL work suggested a maximum of 0.4 wt.% was necessary to avoid complications with PWHT and the AC1 transformation temperatures while still achieving adequate tempering. Table 8 and Figure 6 compare transition temperature with nickel and manganese content. Recent work at ORNL examining the martensite start/finish temperatures has identified a potential and significant correlation of these temperatures to nickel content.
Where nickel is elevated toward the upper end of the range, approximately 18% of the austenite may be retained at 2040C (4000F) and the Mf may actually be below room
temperature! Many authorities recommended that you must allow the component to cool to
~1000C (~2000F) before PWHT to minimize the amount of retained austenite in the weldment.
(20) It was shown by Santella, et al, that weld deposit specimens that were only cooled to 200C and had untempered martensite actually exhibited lower creep rates and relatively long rupture lives. These studies further suggest that nickel has the greatest effect in determining actual Ms and Mf temperatures. On the other hand, for typical base metals and low nickel bearing weld metal, the Mf is high enough in temperature that complete transformation should occur even when maintaining preheat temperatures around 200C (400F) after welding. (36)
0.00 0.50 1.00 1.50 2.00 2.50
Ni + Mn
1350 1400 1450 1500 1550 1600
AC1, Degrees F
730 750 770 790 810 830 850 870
AC1, Degrees C
Effect of Ni + Mn on AC1
P91 Weld Metal
Figure 10. Effect of Ni+Mn on the AC1.
Table 8. Calculated and measured lower critical temperatures (AC1) as a function of Ni + Mn . (3,4,21)
Ni Mn Ni + Mn AC1b 0
0.3 0.51 0.81 1490 *
0.33 0.49 0.82 1499 
0.70 0.37 1.07 1458 
0.71 0.43 1.14 1465 
0.52 0.66 1.18 1454 *
0.70 0.65 1.35 1468 
0.63 0.76 1.39 1436 *
0.79 0.60 1.39 1467 
0.8 1.05 1.85 1416 
1.0 1.3 2.3 1380 
* ORNL Calculation
Variations in vanadium, carbon and nitrogen have been found to have smaller influences on toughness. Manganese is typically controlled at a higher level than the parent material to aid deoxidation and provide a sound weld deposit. However, some users, such as GEC- Alstom, limit Mn + Ni to 1.5% maximum as a safeguard against austenite reformation at the highest PWHT temperatures. Even with Ni + Mn levels consistantly at 1.5 wt.%, Figure 10 suggests that the lower critical temperature could be as low as 7800C (14360F). Standard consumables are normally manufactured within this limit, but to ensure sufficient manganese for effective
deoxidation, the nickel level is lowered to about 0.5 wt.%. However, the average toughness is usually somewhat lower. Toughness can be further reduced when users specify that both Mn and Ni in the weld metal must be in accordance with base metal limits. In order to be sure what effect the PWHT may have on the composition, the ACTUAL composition of the weld filler metal used should be known. Therefore, welding consumables should be procured with actual chemical compositions; e.g. Certified Material Test Reports (CMTR’s) if domestic and/or an EN10204 3.1B certificate from Europe.
What is unknown at this time is the effect of only having a minor portion of a weldment, such as the root and hot pass, at one composition or nickel level and the remainder of the weldment completed with another or lower nickel composition.
Silicon is an essential deoxidant required in both parent and weld metal. Combined with chromium, silicon may also contribute, to a minor degree, to the alloy’s oxidation resistance.
However, although some specifications have effectively the same range as P91 parent material (0.20 - 0.50%Si), a low level of silicon benefits weld metal toughness. The AWS specification limit of 0.30% is lower than the parent material and is perhaps too restrictive for certain consumables, particularly bare wires used with gas shielded processes. Chemical composition, particularly deoxidation tendency of the wire (Figure 11.), also has a significant effect on the welding operability of the GMAW process.(16) A silicon level of about 0.35 wt.% appears to be necessary for satisfactory operating behavior of the metal cored wire and up to 0.50 wt.%
for FCAW wires. These silicon levels have not introduced any known problems in bare wires, SMAW or SAW used in Europe. In fact, silicon levels in bare wire between 0.3 and 0.35 actually aid deoxidation, wetting and manipulation of the puddle for GTAW. The proposed revision of AWS A5.29 to incorporate “-B9” FCAW, expands the silicon range up to 0.5 wt.
percent to further enhance deoxidation.
Sulfur, Phosphorus & Residual Elements
Control of sulfur, phosphorous and residual elements is important. By observing the AWS
"-B9" 0.010 maximum wt.% for sulfur and phosphorus, problems including crater cracking, maintenance of toughness after PWHT or other undesirable grain boundary effects can be avoided in SMAW, GTAW and SAW. It has been found that consumables exhibiting
manganese to sulfur ratios greater than 50 provides one "rule of thumb", when combined with low phosphorous, to avoid crater cracking phenomena. By requiring low phosphorus levels, other elements in trace quantities that "come along for the ride" and that have been shown to be detrimental are also reduced. But, some sulfur (0.003 to 0.005 wt.%) and phosphorus (< 0.010 wt.%) are necessary to promote proper wetting action of the molten puddle where bare wire and gas shielding is used. Elevated levels of phosphorus up to 0.02 wt. % have been found to be permissible for FCAW wires because of the interaction of their slag formers and cooling rates on the deposited metal. Data also suggests that SMAW can normally tolerate this level of phosphorus (approved in European specifications). Where carbon and niobium
(columbium) are both toward the upper end of their respective ranges, tolerance for
phosphorus, sulfur and other trace elements is significantly reduced and may result in crater cracking, hot cracking or other undesirable grain boundary phenomena.
residual elements to maintain resistance from temper embrittlement and elevated toughness of the material. Even though temper embrittlement criteria is not an issue for P91 consumables or most power piping, requiring that they meet an X Factor < 15, as calculated with the Bruscato Formula (or "X-Factor"; where, X = (10P+5Sb+4Sn+As)ppm/100, is a way to reduce or substantially minimize the presence of problematic constituants – primarily phosphorus and tin.
By invoking this requirement, purity is maintained and tendancies that support hot cracking are reduced. The effect of selected chemical elements on creep resistance and toughness are summarized in Table 9.
Figure 11. Effect of Oxygen Content on Toughness for Selected P91 Weldments. (16)
Table 9. Effect Summary of Individual Elements on P91 Weld Metal (2,3,6,13,16,20)
Element Effect on Creep Resistance Effect on Toughness Notes Ni
CE believed that a negative effect on creep strength would be observed above 0.4 wt. percent.
Increases toughness. Europeans request up to 0.8 wt. % for increased toughness.
None Decreasing Mn will slightly improve
toughness, but Mn is necessary for deoxidation of the molten weld pool. A minimum level of 0.40 wt. % is recommended.
Stated range required. Variation within the range required for creep resistance result in little change.
Stated range required. N/A Si
N/A As silicon decreases toughness increases.
Silicon must remain above 0.15 wt. % to provide molten pool deoxidation and prevention of porosity. Preheat temperature to avoid cracking also increases with silicon content. Silicon therefore should be maintained as low as practically possible.
Data suggests that levels between 0.20 and 0.50 wt. % are acceptable.
Minimal Cb(Nb) required to maintain creep properties.
Elevated Cb(Nb) significantly lowers toughness. 0.025 to 0.050 wt. % has been found to be acceptable.
Minimal levels required to Maintain creep properties.
Vanadium above 0.25 wt. % significantly lowers toughness.
Minimal levels required to form carbonitrides to enhance creep properties.
High nitrogen levels lower toughness via formation of nitrides with other elements such as aluminum.
Al N/A Limitations imposed in “-B9” specifications
to avoid formation of toughness lowering nitrides.
A minimum of 0.08 wt.% is required to achieve adequate creep strength.
Lower carbon can significantly increase toughness.
1. CE concerns about elevated nickel content have not been verified. The widespread use and success of the higher nickel versions by the Europeans suggest that such concerns have not been validated.
2. Austenite forming elements Ni and Mn must be adjusted to ensure that the AC1 temperature is not below the PWHT temperature. Failure to do so may promote austenite formation which can lead to untempered martensite during cooling and result in lower creep properties. Therefore, as nickel is increased, manganese may have to decrease. Ni + Mn less than 1.5 is a guideline followed by European users.
3. Where carbon and niobium are both toward the upper end of their respective ranges, tolerance for phosphorus, sulfur and other trace elements is significantly reduced and may result in crater cracking, hot cracking or other undesirable grain boundary phenomena.
4. Chemistry range shown for each element is maximum and will vary depending on product form.
Application of elevated preheat and PWHT, including interpass temperature controls, are absolutely necessary with Grade 91 weldments, regardless of diameter or thickness. The literature suggests that 200oC (~ 400oF) is adequate for preheating P91 weldments.
Fabricators typically aim for 250oC (~ 500oF) but will go as low as 150oC (~ 300oF), for root and hot pass layers only, thin-walled components or where GTAW is utilized. (8,22)
Interpass temperatures normally are restricted to 300 to 3500C (600-7000F). Field operations rarely have problems with interpass temperature limitations on heavy sections. Shop
operations using SAW typically will exceed interpass temperatures and require cooling between passes. 3500C (7000F) appears to the upper practical temperature because of bead shape control limitations.
• PWHT is one of the single most important factors in producing satisfactory weldments in P(T)91 materials. The PWHT methodology and implementation must be verified to ensure that the weldments are ACTUALLY receiving PWHT at the proper temperature. Additional thermocouples or qualification testing may be required.
Proper tempering of the martensitic microstructure is essential for obtaining reasonable levels of toughness. In practice this involves selecting both an appropriate temperature and time.
The AWS specification for consumable classification requires PWHT of 730-7600C (1346- 1400 0F) for 1 hour. This time requirement is inadequate for normal fabrication procedures of heavywall components. Table 10 shows how mechanical properties vary with time at
temperature. A minimum of 2-3h at temperature in the range 750-7600C (1382-1418 0F) is required, or longer for thicker sections. This temperature-time aspect is recognized by EN 1599 which specifies a PWHT requirement of 750-7700C for 2-3h for welding consumables.
However, it is important to limit PWHT temperature to avoid the risks of austenite
reformation and the transformation to fresh untempered martensite, particularly in weld metal with elevated nickel. (16,18, 35, 36)
Caution must also be observed when conducting PWHT on thin sections (< 10mm; 0.375 in.).
Data suggests that 15 to 30 minutes at 760C (1400F) is adequate for satisfactory tempering of thin section weldments. In the absence of specific empirical data, sections over 10mm (0.375 in.) should receive two hours of PWHT, minimum, to achieve proper tempering.
Table 10. Mechanical properties resulting from different times for E9015-B9 PWHT @ 7600C (14000F) (23)
CVN ft-bs@680F As –Welded
210 [119 @ 10220F]
- - 3
45 120.3 101.8 17 13
120 [240-260 HV10]
104.7 83.5 23 53
The effect of extended time and PWHT on toughness and hardness are further presented in Figures 12 and 13. It has been suggested that 760oC (~1400 oF) is the optimum PWHT temperature, pending heating equipment capability and nickel content of the welding filler metals. And, even though codes permit less time, PWHT should be conducted for a minimum of two (2) hours at temperature, even for weld metal testing, to provide sufficient tempering.
Figure 12. Influence of PWHT Time and Temperature on Toughness (2,10)
Figure 13. Influence of PWHT Time and Temperature on Hardness.(2,10)
7040C (13000F) to 7600C (14000F) range specified in Table 132. Interpretation 24-5 offered the following: (24)
Subject: B31.1 Table 132, Postweld Heat Treatment Date Issued: October 27, 1993
Question: Is it permissible to postweld heat treat SA-182 F91 materials at 14000F- 14500F instead of 13000F-14000F as specified for P-No. 5 in Table 132?
Reply: Yes, provided the lower critical temperature of the SA-182 F91 material is not exceeded. See Para. 132.2(A).
Figure 14 presents typical preheat, welding/interpass and PWHT schedules for P91 to P91.
This figure illustrates cooling the weldments to room temperature prior to post weld heat treat to permit complete transformation to a martensitic structure. On large vessels and heavy-wall piping, this is not always practical. Successful practice over two decades has shown that satisfactory results can be obtained by allowing the completed weld to cool to the preheat temperature and holding this temperature continuously up to initiation of the post weld heat treat. Success is dependent on close attention to maximum interpass temperatures and time at temperature during the final post weld heat treat. As mentioned earlier, further investigation is needed to clarify this difference in methodology. Conversely, it was absolutely necessary to cool to room temperature prior to post weld heat treatment where X20 materials were involved. Thus, this flexibility offered by P91 materials is much more attractive to fabricators and installers. (9,18,19,20,35,36)
Also of critical importance on heavy sections, may be implementation of a post weld bake when using flux-type processes. This bake should be at least at the preheat temperature if the fabrication schedule requires the weldment to cool to room
temperature in process or prior to application of post weld heat treatment. Post bake times and temperatures vary from 4 hours at 2600C (5000F) to only 15 minutes at 3160C (6000F). Success with this much variation is due to the advances made in consumable formulation and implementation of proper preheat, welding, welding consumable storage and handling practices.
Methods available for preheat, post baking and post weld heat treatment vary in ease of use, complexity and effectiveness. Approaches include furnace, flame, electrical resistance heating and electrical induction heating. Each approach exhibits specific implementation and technical characteristics. These are further discussed in Pratical Considerations, Para. 7.1.
200 400 600 800 1000
400 - 500 F 200-250 C Weld Preheat
1375 - 1425 F 745 - 775 C
PWHT Heating Rate
100 - 150 C/h 180 - 270 F/h
Cooling Rate 150 - 200 C/h 270 - 400 F/h
Below 400 C / 750 F Cool in Still Air
80 - 100 C 175 - 212 F
Figure 14. Typical thermal cycles observed during welding and PWHT. (9,25)
4.3.3 Welding Process Effects
Mechanical property results vary with welding process. This is especially true for processes that rely on fluxes and slag systems for alloying and/or shielding gases for protection of the molten weld pool. Primary factors that can affect weld metal properties include: heat input versus amount of weld metal deposited, grain size produced versus bead shape, and influences from wetting agents, crack inhibitors, deoxidizers and slag formers as they affect gas levels, microalloying and introduction of tramp or residual elements for the SMAW, FCAW and SAW processes.
Reductions in mechanical properties, primarily toughness, as a function of welding process are summarized in Table 11.
(GTAW = 100% of achievable properties) Welding
Typical Toughness Reduction
Wetting Agents, Crack Inhibitors, Deoxidizers or Slag Formers
GTAW None Si, Mn, Ti
SAW 25-50% SiO2, MnO3, etc.
SMAW 40-50% CaCO2, etc.
FCAW 50-70% Varies
During original development of the Grade 91 SMAW consumable and in later
manufacture, it was found that even though a lot of electrodes had proper chemistry, tramp elements and coating variables could actually result in an electrode that exhibited nil ductility. Thus, mechanical testing, including tensile and impact tests, is
recommended on a lot to lot, per size per diameter basis, to ensure that the proper material has been produced and supplied.
4.3.4 Bead Shape and Position Effect
Bead shape and welding position have a significant effect on toughness. Most test data is reported in the flat welding position (1G). Bead shape plays an important role as shown in Figure 15. Thin, wide beads that permit some degree of tempering from the heat of welding induce grain refinement on previously deposited metal. Thicker bead cross-sections minimize grain refinement. Loss of toughness is normally observed in the vertical (3G) and overhead (4G) positions with SMAW– mostly due to the bead shape in the weldment. Even with an elevated weld metal nickel content (0.76 wt.%) to enhance toughness, the effect of position and corresponding bead shape and inability to provide tempering or induce grain refinement is evident and is as shown in Figures 15 and 16. However, some new FCAW wires have shown improvent in toughness in out-of-position welding. Increased interbead tempering is believed to be the cause. (19)
Figure 15. Influence of Bead Shape on Weld Metal Toughness for Typical FCAW and SAW Applications. (2,19,23)
Figure 16. Effect of Welding Position on Toughness for SMAW. (2) 4.3.5 Toughness Testing Temperature
It must also be noted that the test temperature used when conducting toughness tests can have a dramatic effect on the results. (3,21) Experimental work has shown that the transition temperature for this alloy hovers around room temperature. Up to a 30 to 50 percent increase in toughness can be observed when tests are performed at 22-230C (72-750F) as opposed to 200C (680F)! (3,4,30)
5.0 DISSIMILAR WELDING
Dissimilar welds involving P91, P11 and P22 and austentic stainless steels are performed on a routine basis. Welds between the low alloy ferritic steels utilize either P91 or materials
matching the lower alloy type base metals. In such weldments, carbon diffusion occurs during the tempering heat treatment due to the difference in chromium content of the materials.
Carbon will migrate from the lower chromium material to the higher chromium one. For example: When P22 (E901X-B3/ER90S-B3/EB3) filler metal is used, the decarburized zone will be in the P22 weld metal next to the P91 with the carburized zone located in the P91 HAZ. If P91 weld metal is used, the carbon depleted zone will be located in the coarse grained P22 HAZ and the carburized zone in the P91 weld metal. The extent of the decarburized zone depend on the tempering temperature and time at temperature. The only way to avoid this condition is to use a nickel-base welding consumable. (9)
Decarburization in these dissimilar weldments typically only affect room temperature toughness properties. Creep rupture properties are usually not affected. (9)
Transitions or dissimilar welds between P91 and austenitic stainless steels normally uses nickel- base weld material. The weld metal can be applied to or involves buttering a P91 "pup" piece that can be heat treated and then field installed. In this manner, one weld can be made and PWHT as a P91 to nickel base while the other a nickel base to stainless steel. (9)
EPRI/RRAC work (39) showed that estimated life was improved considerably for DMW’s where P91 was buttered with E9018-B3, the butter subjected to a PWHT 7600C (14000F), then the final weld completed to the P22 followed by PWHT at 6770C (12500F) to 7040C (13000F). This technique produced results that were approximately two times greater than a DMW that is completed without the buttering step. The improvement was believed to be due to improvement of the HAZ from the butter PWHT and has a projected service life of
approximately 350,000 hours. Further, conducting PWHT at 7320C (13500F) versus 6770C (12500F) on E9018-B3 for DMW’s resulted in substantially better projected service life. This work showed that use of E9018-B3 weld metal for P91 to P22 DMW’s is both prudent and sufficiently adequate.
Additional tests were conducted using nickel-base filler metal (ENiCrFe-3) in both a
buttered/non-buttered sequence with similar results for a buttered-multiple PWHT approach.
Due to recent service failures (40) identified with using ENiCrMo-3 for selected P91 DMW’s, it is recommended that ENiCrFe-2 or –3 filler metals be used until further work is completed.
Table 12 illustrates projected results from the recent EPRI/RRAC work on DMW’s. (39)
Table 12. Estimated Remaining Life at 5660C (10500F) based on experimental results and extrapolation of Isostress Curves. (39)
@ 5660C (10500F) and 52.8 MPa (7.8 ksi)
Weldment PWHT 6770C (12500F)
Weldment PWHT 7320C (13500F)
E9018-B3 53,158 347,809
E9018-B3 w/butter PWHT @ 7600C (14000F) 551,445 642,573
ENiCrFe-3 177,017 122,484
ENiCrFe-3 w/butter PWHT @ 7600C (14000F) 362,446 293,892
1. Stress rupture test coupons were centered on P91-side of weld joint and includes base, HAZ, butter (if present) and weld metal. No P22 base metal was included in the test specimens.
2. Cross-weld stress rupture tests were performed for ENiCrFe-3 weldments resulting in specimen failures within the P22 HAZ.
Extreme care and planning must be observed concerning post weld heat treatment of dissimilar weldments involving P91. "Pup" pieces or multiple buttering/PWHT operations may be required when joining P91 to P11 or low carbon steels because tempering temperatures necessary for P91 may exceed lower transformation temperatures for some of the lower strength alloys. In these cases, P91 is oftentimes buttered with P22 or -B3 (or lower) type
weld metal, PWHT at P91 temperatures, then the field weld is made with the lower strength alloy, followed by a subsequent PWHT a temperatures appropriate to the lower alloy.
Typical dissimilar weld (DMW) combinations and corresponding approaches are presented in Table 13. Weld filler metal selection possiblities for DMW’s are shown in Table 14.
Guideline PWHT temperatures are included in Table 15. In most cases, use of the lower strength weld metal is recommended. The temperatures shown, particularly where B9 weld metal is involved, are selected to provide proper tempering of the weld metal. These
temperatures may not necessarily coincide with traditional code values and may require specific knowledge of the transformation temperatures or special properties of the materials involved and additional welding procedure qualifications. For example, ENiCrMo-3 (“625”) should NOT be used because it will embrittle at the PWHT temperatures required for Grade 91.
Table 13. Dissimilar Weld Combinations and Approach (9, 22)
P91 to P22 B3 & PWHT @ 13500F P91 to P11 Butter P91 w/B2 & PWHT @
13500F; Then, join w/B2 &
PWHT @ 11000F P91 to SS Butter P91 w/Ni & PWHT @
14000F; Then join to SS w/Ni
Table 14. Dissimilar Welding Filler Metal Selection (9, 22,26,27)
P(T) 11 22 23 91 911 92 SS
11 B2 B2 B2 B2 B2 B2 309
22 B2 B3 B3,G B3 B3,G B3,G 309,Ni
23 B2 B3,G
B3,G,Ni G,Ni W,G
W,G, B9 G,Ni,SS
91 B2 B3 G, Ni B9 W,B9,G W,G, B9 Ni
911 B2 B3,G W,G W,B9,G W,G
W, G, B9 Ni
92 B2 B3,G
B, W,B9, G
W,G,B9 B,W,G Ni
SS 309 309,Ni G,Ni,SS Ni Ni Ni SS,Ni
G = Nonstandard composition B2 = 1-1/4 Cr ½ Mo
B3 = 2-1/4Cr 1 Mo B9 = 9 Cr 1 Mo V W = Tungsten Modified B = Boron Modified, etc.
Ni = Nickel Base (ENiCrFe-2 or –3)
SS = Stainless, 308H, 309H, 316H, 347H, 16-8-2 Butter or buffer layers may be required.
NOTE: ENiCrMo-3 (“625”) should NOT be used because it will embrittle at the PWHT temperatures required for Grade 91.
Table 14 selections are options based on current technology or practice. Other filler metals may be necessary depending upon service conditions, buttering and overall PWHT
Table 15. Recommended PWHT Temperatures (0F) for Dissimilar Welds (9,22,26,27)
P(T) 11 22 23 91 911 92 SS
11 1350 + 25 1350 + 25
Butter 11 1350 + 25
Butter 91 1375 + 25;
1275 + 25
Butter 911 1375 + 25;
1275 + 25
Butter 92 1375 + 25;
1275 + 25
Butter 11 (opt) 1275 + 25
22 1350 + 25 1350 + 25
1350 + 25 1375 + 25 1375 + 25 1375 + 25
Butter (opt) 1350 + 25
Butter 11 1350 + 25
1350 + 25 None
Butter 91 1375 + 25
Butter 911 1375 + 25
1375 + 25 None
Butter 91 1375 + 25;
1275 + 25
1375 + 25
1375 + 25 1400 + 25 1375 + 25 1375 + 25
Butter 91 1375 + 25
Butter 911 1375 + 25;
1275 + 25
1375 + 25
1375 + 25 1375 + 25 1375 + 25 1375 + 25
Butter 911 1375 + 25
Butter 92 1375 + 25;
1275 + 25
1375 + 25
1375 + 25 1375 + 25 1375 + 25 1375 + 25
Butter 92 1375 + 25
Butter 11 (opt) 1275 + 25
1350 + 25 None
Butter 91 1375 + 25
Butter 911 1375 + 25
1375 + 25 None
1. The recommendations in the above table were developed from References 9,22,26 & 27.
2. The objective in dissimilar welding is to maintain properties while addressing differences in the respective base metals, HAZ’s and PWHT temperatures. See Table 14 for weld metals.
3. Buttering and multi-step PWHT is used where PWHT required for one base metal, HAZ or weld metal is excessive for one or more of the others.
4. Where “Butter” is shown, “Butter” the indicated base metal, perform PWHT of the butter at the temperature listed, then join the other material to the butter and perform PWHT of the completed weldment at the second temperature.
5. T23 has shown tendancies toward reheat cracking from PWHT. This alloy was originally designed to be used without PWHT. Thus, buttering may be required.
6. T24 typically does not require PWHT. Thus, buttering may be required.
7. Caution must be observed when selecting PWHT temperatures that will not encroach on the AC1 of the lowere temperature material.
8. Where B9 weld metal is used for buttering or joining, 1400 + 25F is the recommended heat treatment temperature.
6.0 WELDING PROCESSES
Welding of P91 can be accomplished with FCAW, GMAW, GTAW, SAW and SMAW processes. Welding filler metals have been formulated to complement the base metal but do require multiple refining operations to achieve the low levels of residual elements, especially phosphorus. A major effort was initiated on a worldwide basis to formulate weld metals that would exhibit friendly weldability while maintaining the required mechanical properties.
Combustion Engineering formulated and tested nearly 200 different SMAW compositions in the original test program – only two or three of the compositions exhibited both satisfactory mechanical properties and welder appeal. (17)
Welding process selection is normally a funciton of thickness, diameter, position and quantity.
Table 16 illustrates typical production rates as a function of welding process. Clearly, the SAW process offers significant potential where it can be used.
Table 16. Typical Manhours for Pipe to Pipe Welds as a Function of Welding Process (37.5 degree V-groove, Schedule 40). (17,28-30))
Manhours per Pipe Size, Diameter Welding
Process 3-inch 6-inch 12-inch 24-inch
GTAW 0.7 1.9 6.4 27.5
SMAW 0.5 1.0 2.8 12.1
FCAW 0.2 0.3 0.8 3.5
SAW N/A 0.1 0.3 1.4
NOTE: Manhours based on average operating factors and deposition rates. Fit-up and groove preparation not included. Estimates based on using single process from root to cap.
6.1 Gas Metal Arc Welding (GMAW)
The situation with GMAW, particularly with active gas mixtures, is more complex because of the variable recovery of key elements such as Mn, Si, and Nb/Cb. Modifications to the compositions of solid or metal cored wires are similar to those applied to covered electrodes and these are beneficial for microstructural control even though toughness may far exceed many specification requirements.
It must be strongly noted that qualification and use of solid wire GMAW should be approached with much caution! The “-B9” composition is lean on deoxidizers, which are important to proper operation and results with GMAW. Because of this, wetting action is reduced and the preponderance for lack of fusion type defects and oxide inclusion content affect the ability to perform successful welding. A few fabricators have qualified GMAW, but few have implemented it into production because of it’s operator specific characteristics and inability to perform in a reproduceable manner.